Synthesis and crystal structure of silicon pernitride SiN2 at 140 GPa
Jurzick, Pascal L.; Krach, Georg; Brüning, Lukas; Schnick, Wolfgang; Bykov, Maxim; Acta Crystallographica Section E Crystallographic Communications 79 (2023) –; doi:10.1107/S2056989023008058

data_2022864
_publ_section_title
;
 Synthesis and crystal structure of silicon pernitride SiN2 at
 140&#x2005;GPa
;
_journal_coeditor_code           WM5694
_journal_issue                   10
_journal_name_full
'Acta Crystallographica Section E Crystallographic Communications'
_journal_paper_doi               10.1107/S2056989023008058
_journal_volume                  79
_journal_year                    2023
_chemical_formula_iupac          'Si N2'
_chemical_formula_moiety         'N2 Si'
_chemical_formula_sum            'N2 Si'
_chemical_formula_weight         56.11
_chemical_name_systematic        'Silicon pernitride'
_space_group_crystal_system      cubic
_space_group_IT_number           205
_space_group_name_Hall           '-P 2ac 2ab 3'
_space_group_name_H-M_alt        'P a -3'
_atom_sites_solution_primary     dual
_audit_creation_method
;
Olex2 1.5
(compiled 2023.03.06 svn.rbb2c1857 for OlexSys, GUI svn.r6748)
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.1205(5)
_cell_length_b                   4.1205(5)
_cell_length_c                   4.1205(5)
_cell_measurement_reflns_used    79
_cell_measurement_temperature    293
_cell_measurement_theta_max      16.4030
_cell_measurement_theta_min      3.4280
_cell_volume                     69.960(15)
_computing_cell_refinement
;
CrysAlisPro (Rigaku OD, 2023)
;
_computing_data_collection
;
CrysAlisPro (Rigaku OD, 2023)
;
_computing_data_reduction
;
CrysAlisPro (Rigaku OD, 2023)
;
_computing_molecular_graphics
;
<i>VESTA</i> (Momma & Izumi, 2011)
;
_computing_publication_material
;
Olex2 (Dolomanov <i>et al.</i>,  2009)
;
_computing_structure_refinement
;
SHELXL (Sheldrick, 2015<i>b</i>)
;
_computing_structure_solution
;
<i>SHELXT</i> (Sheldrick, 2015<i>a</i>)
;
_diffrn_ambient_temperature      293
_diffrn_detector_area_resol_mean 5.0
_diffrn_measured_fraction_theta_full 0.955
_diffrn_measured_fraction_theta_max 0.732
_diffrn_measurement_device       'abstract diffractometer'
_diffrn_measurement_device_type  'customized \w-circle diffractometer'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  synchrotron
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.28457
_diffrn_reflns_av_R_equivalents  0.0490
_diffrn_reflns_av_unetI/netI     0.0531
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -4
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            269
_diffrn_reflns_theta_full        9.831
_diffrn_reflns_theta_max         18.450
_diffrn_reflns_theta_min         3.429
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    0.214
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.74987
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
(CrysAlisPro; Rigaku OD, 2023)
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    5.327
_exptl_crystal_description       irregular
_exptl_crystal_F_000             112
_exptl_crystal_size_max          0.001
_exptl_crystal_size_mid          0.001
_exptl_crystal_size_min          0.001
_refine_diff_density_max         1.079
_refine_diff_density_min         -1.146
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.072
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     6
_refine_ls_number_reflns         101
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.072
_refine_ls_R_factor_all          0.1285
_refine_ls_R_factor_gt           0.0706
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1090P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1601
_refine_ls_wR_factor_ref         0.1907
_reflns_number_gt                60
_reflns_number_total             101
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            wm5694sup1.cif
_cod_data_source_block           I
_cod_original_cell_volume        69.96(3)
_cod_database_code               2022864
_shelx_estimated_absorpt_t_min   1.000
_shelx_estimated_absorpt_t_max   1.000
_shelx_hkl_checksum              28902
_shelx_res_file                  {26c6c36b-09aa-4389-a52a-17eac477c28c
_shelx_res_checksum              52692
_cod_database_fobs_code 2022864